Superconductivity
Peter Schm¨user
Institut f¨ur Experimentalphysik der Universit¨at Hamburg
Abstract
Lowtemperature superconductivity is treated at an introductory level.The
topics include MeissnerOchsenfeld effect and London equations,thermody
namic properties of the superconducting state,type I and II superconductors,
ﬂux quantisation,superconductors in microwave ﬁelds and superconducting
quantum interference effects.Important experiments are discussed.The basic
ideas of the BCS theory and its implications are outlined.
1.INTRODUCTION
In these lectures I want to give an introduction into the physical principles of superconductivity and its
fascinating properties.More detailed accounts can be found in the excellent text books by W.Buckel
[1] and by D.R.Tilley and J.Tilley [2].Superconductivity was discovered [3] in 1911 by the Dutch
physicist H.Kamerlingh Onnes,only three years after he had succeeded in liquefying helium.During his
investigations on the conductivity of metals at low temperature he found that the resistance of a mercury
sample dropped to an unmeasurably small value just at the boiling temperature of liquid helium.The
original measurement is shown in Fig.1.Kamerlingh Onnes called this totally unexpected phenomenon
‘superconductivity’ and this name has been retained since.The temperature at which the transition took
place was called the critical temperature T
c
.Superconductivity is observed in a large variety of materials
but,remarkably,not in some of the best normal conductors like copper,silver and gold,except at very
high pressures.This is illustrated in Fig.2 where the resistivity of copper,tin and the ‘hightemperature’
superconductor YBa
2
Cu
3
O
7
is sketched as a function of temperature.Table 1 lists some important
superconductors together with their critical temperatures at vanishing magnetic ﬁeld.
Fig.1:The discovery of superconductivity by Kamerlingh Onnes.
Fig.2:The lowtemperature resistivity of copper,tin and YBa
2
Cu
3
O
7
.
Table 1:The critical temperature of some common materials at vanishing magnetic ﬁeld.
material
Ti
Al
Hg
Sn
Pb
Nb
NbTi
Nb
3
Sn
T
c
[K]
0:4
1:14
4:15
3:72
7:9
9:2
9:2
18
A conventional resistance measurement is far too insensitive to establish inﬁnite conductivity,
a much better method consists in inducing a current in a ring and determining the decay rate of the
produced magnetic ﬁeld.A schematic experimental setup is shown in Fig.3.A bar magnet is inserted
in the still normalconducting ring and removed after cooldown below T
c
.The induced current should
decay exponentially
I(t) = I(0) exp(t=)
with the time constant given by the ratio of inductivity and resistance, = L=R,which for a normal
metal ring is in the order of 100 s.In superconducting rings,however,time constants of up to 10
5
years
have been observed [4] so the resistance must be at least 15 orders of magnitude belowthat of copper and
is indeed indistinguishable from zero.An important practical application of this method is the operation
of solenoid coils for magnetic resonance imaging in the shortcircuit mode which exhibit an extremely
slow decay of the ﬁeld of typically 3 10
9
per hour [5].
Fig.3:Induction of a persistent current in a superconducting ring.
There is an intimate relation between superconductivity and magnetic ﬁelds.W.Meissner and R.
Ochsenfeld [6] discovered in 1933 that a superconducting element like lead completely expelled a weak
magnetic ﬁeld from its interior when cooled below T
c
while in strong ﬁelds superconductivity broke
down and the material went to the normal state.The spontaneous exclusion of magnetic ﬁelds upon
crossing T
c
could not be explained in terms of the Maxwell equations and indeed turned out to be a
nonclassical phenomenon.Two years later,H.and F.London [7] proposed an equation which offered
a phenomenological explanation of the MeissnerOchsenfeld effect but the justiﬁcation of the London
equation remained obscure until the advent of the Bardeen,Cooper and Schrieffer theory [8] of super
conductivity in 1957.The BCS theory revolutionized our understanding of this fascinating phenomenon.
It is based on the assumption that the supercurrent is not carried by single electrons but rather by pairs of
electrons of opposite momenta and spins,the socalled Cooper pairs.All pairs occupy a single quantum
state,the BCS ground state,whose energy is separated from the singleelectron states by an energy gap
which in turn can be related to the critical temperature.The BCS theory has turned out to be of enormous
predictive power and many of its predictions and implications like the temperature dependence of the en
ergy gap and its relation to the critical temperature,the quantisation of magnetic ﬂux and the existence
of quantum interference phenomena have been conﬁrmed by experiment and,in many cases,even found
practical application.
A discovery of enormous practical consequences was the ﬁnding that there exist two types of
superconductors with rather different response to magnetic ﬁelds.The elements lead,mercury,tin,alu
minium and others are called ‘type I’ superconductors.They do not admit a magnetic ﬁeld in the bulk
material and are in the superconducting state provided the applied ﬁeld is below a critical ﬁeld H
c
which
is a function of temperature.All superconducting alloys like leadindium,niobiumtitanium,niobiumtin
and also the element niobium belong to the large class of ‘type II’ superconductors.They are charac
terized by two critical ﬁelds,H
c1
and H
c2
.Below H
c1
these substances are in the Meissner phase with
complete ﬁeld expulsion while in the range H
c1
< H < H
c2
a type II superconductor enters the mixed
phase in which magnetic ﬁeld can penetrate the bulk material in the form of ﬂux tubes.The Ginzburg
Landau theory [9] provides a theoretical basis for the distinction between the two types.Around 1960
Gorkov [10] showed that the phenomenological GinzburgLandau theory is a limiting case of the BCS
theory.Abrikosov [11] predicted that the ﬂux tubes in a type II superconductor arrange themselves in
a triangular pattern which was conﬁrmed in a beautiful experiment by Essmann and Tr¨auble [12].In
1962 Josephson [13] studied the quantum theoretical tunnel effect in a system of two superconductors
separated by a thin insulating layer and he predicted peculiar and fascinating properties of such a Joseph
son junction which were all conﬁrmed by experiment and opened the way to superconducting quantum
interference devices (SQUID’s) with extreme sensitivity to tiny magnetic ﬁelds.
2.MEISSNEROCHSENFELDEFFECT ANDLONDONEQUATION
We consider a cylinder with perfect conductivity and raise a magnetic ﬁeld fromzero to a ﬁnite value H.
A surface current is induced whose magnetic ﬁeld,according to Lenz’s rule,is opposed to the applied
ﬁeld and cancels it in the interior.Since the resistance is zero the current will continue to ﬂow with
constant strength as long as the external ﬁeld is kept constant and consequently the bulk of the cylinder
will stay ﬁeldfree.This is exactly what happens if we expose a lead cylinder in the superconducting
state (T < T
c
) to an increasing ﬁeld,see the path (a)!(c) in Fig.4.So below T
c
lead acts as a perfect
diamagnetic material.There is,however,another path leading to the point (c).We start with a lead
cylinder in the normal state (T > T
c
) and expose it to a ﬁeld which is increased from zero to H.Eddy
currents are induced in this case as well but they decay rapidly and after a few hundred microseconds
the ﬁeld lines will fully penetrate the material (state (b) in Fig.4).Now the cylinder is cooled down.
At the very instant the temperature drops below T
c
,a surface current is spontaneously created and the
magnetic ﬁeld is expelled from the interior of the cylinder.This surprising observation is called the
MeissnerOchsenfeld effect after its discoverers;it cannot be explained by the law of induction because
the magnetic ﬁeld is kept constant.
Fig.4:Alead cylinder in a magnetic ﬁeld.Two possible ways to reach the superconducting ﬁnal state with H > 0 are sketched.
Ideally the length of the cylinder should be much larger than its diameter to get a vanishing demagnetisation factor.
In a (T;H) plane,the superconducting phase is separated from the normal phase by the curve
H
c
(T) as sketched in Fig.5.Also indicated are the two ways on which one can reach the point (c).It
is instructive to compare this with the response of a ‘normal’ metal of perfect conductivity.The ﬁeld
increase along the path (a)!(c) would yield the same result as for the superconductor,however the
cooldown along the path (b)!(c) would have no effect at all.So superconductivity means deﬁnitely
more than just vanishing resistance.
Fig.5:The phase diagramin a (T;H) plane.
I have already used the terms ‘superconducting phase’ and ‘normal phase’ to characterize the
two states of lead.These are indeed phases in the thermodynamical sense,comparable to the different
phases of H
2
O which is in the solid,liquid or gaseous state depending on the values of the parameters
temperature and pressure.Here the relevant parameters are temperature and magnetic ﬁeld (for some
materials also pressure).If the point (T;H) lies below the curve H
c
(T) the material is superconducting
and expels the magnetic ﬁeld,irrespective of by which path the point was reached.If (T;H) is above
the curve the material is normalconducting.
The ﬁrst successful explanation of the MeissnerOchsenfeld effect was achieved in 1935 by Heinz
and Fritz London.They assumed that the supercurrent is carried by a fraction of the conduction electrons
in the metal.The ‘superelectrons’ experience no friction,so their equation of motion in an electric ﬁeld
is
m
e
@~v
@t
= e
~
E:
This leads to an accelerated motion.The supercurrent density is
~
J
s
= en
s
~v
where n
s
is the density of the superelectrons.This immediately yields the equation
@
~
J
s
@t
=
n
s
e
2
m
e
~
E:(1)
Now one uses the Maxwell equation
~
r
~
E =
@
~
B
@t
and takes the curl (rotation) of (1) to obtain
@
@t
m
e
n
s
e
2
~
r
~
J
s
+
~
B
= 0:
Since the time derivative vanishes the quantity in the brackets must be a constant.Up to this point the
derivation is fully compatible with classical electromagnetism,applied to the frictionless acceleration of
electrons.An example might be the motion of electrons in the vacuumof a television tube or in a circular
accelerator.The essential new assumption H.and F.London made is that the bracket is not an arbitrary
constant but is identical to zero.Then one obtains the important London equation
~
r
~
J
s
=
n
s
e
2
m
e
~
B:(2)
It should be noted that this assumption cannot be justiﬁed within classical physics,even worse,in
general it is wrong.For instance the current density in a normal metal will vanish when no electric ﬁeld is
applied,and whether a static magnetic ﬁeld penetrates the metal is of no importance.In a superconductor
of type I,on the other hand,the situation is such that Eq.(2) applies.Combining the fourth Maxwell
equation (for timeindependent ﬁelds)
~
r
~
B =
0
~
J
s
and the London equation and making use of the relation
~
r(
~
r
~
B) = r
2
~
B
(this is valid since
~
r
~
B = 0) we get the following equation for the magnetic ﬁeld in a superconductor
r
2
~
B
0
n
s
e
2
m
e
~
B = 0:(3)
It is important to note that this equation is not valid in a normal conductor.In order to grasp the signiﬁ
cance of Eq.(3) we consider a simple geometry,namely the boundary between a superconducting half
space and vacuum,see Fig.6a.Then,for a magnetic ﬁeld parallel to the surface,Eq.(3) becomes
d
2
B
y
dx
2
1
2
L
B
y
= 0
with the solution
B
y
(x) = B
0
exp(x=
L
):
Here we have introduced a very important superconductor parameter,the London penetration depth
L
=
r
m
e
0
n
s
e
2
:(4)
So the magnetic ﬁeld does not stop abruptly at the superconductor surface but penetrates into the material
with exponential attenuation.For typical material parameters the penetration depth is quite small,20 –
50 nm.In the bulk of a thick superconductor there can be no magnetic ﬁeld,which is just the Meissner
Ochsenfeld effect.Here it is appropriate to remark that in the BCS theory not single electrons but pairs
of electrons are the carriers of the supercurrent.Their mass is m
c
= 2m
e
,their charge 2e,their density
n
c
= n
s
=2.Obviously the penetration depth remains unchanged when going from single electrons to
Cooper pairs.
We have now convinced ourselves that the superconductor can tolerate a magnetic ﬁeld only in a
thin surface layer (this is the case for type I superconductors).An immediate consequence is that current
ﬂow is restricted to the same thin layer.Currents in the interior are forbidden as they would generate
magnetic ﬁelds in the bulk.The magnetic ﬁeld and the current which are caused by an external ﬁeld
parallel to the axis of a lead cylinder are plotted in Fig.6b.Another interesting situation occurs if we
pass a current through a lead wire (Fig.6c).It ﬂows only in a very thin surface sheet of about 20 nm
thickness,so the overall current in the wire is small.This is a ﬁrst indication that type I superconductors
are not suitable for winding superconducting magnet coils.
Fig.6:(a) Exponential attenuation of a magnetic ﬁeld in a superconducting half plane.(b) Shielding current in a superconduct
ing cylinder induced by a ﬁeld parallel to the axis.(c) A currentcarrying wire made froma type I superconductor.
The penetration depth has a temperature dependence which can be calculated in the BCS theory.
When approaching the critical temperature,the density of the supercurrent carriers goes to zero,so
L
must become inﬁnite:
L
!1 for T!T
c
:
This is shown in Fig.7.An inﬁnite penetration depth means no attenuation of a magnetic ﬁeld which is
just what one observes in a normal conductor.
Fig.7:Temperature dependence of the London penetration depth.
3.THERMODYNAMICPROPERTIES OF SUPERCONDUCTORS
3.1 The superconducting phase
A material like lead goes from the normal into the superconducting state when it is cooled below T
c
and
when the magnetic ﬁeld is less than H
c
(T).It has been mentioned already that this is a phase transition
comparable to the transition from water to ice at 0
C and normal pressure.Phase transitions take place
when the new state is energetically favoured.The relevant thermodynamic energy is here the Gibbs free
energy (see Appendix A)
G = U T S
0
~
M
~
H (5)
where U is the internal energy,S the entropy and M the magnetisation of the superconductor (the
magnetic moment per unit volume).A measurent of the free energy of aluminium is shown in Fig.8a.
Below T
c
the superconducting state has a lower free energy than the normal state and thus the transition
normal!superconducting is associated with a gain in energy.The entropy of the superconducting state
is lower because there is a higher degree of order in this state.Fromthe point of view of the BCS theory
this is quite understandable since the conduction electrons are paired and collect themselves in a single
quantum state.Numerically the entropy difference is small,though,about 1 milliJoule per mole and
Kelvin,from which one can deduce that only a small fraction of the valence electrons of aluminium is
condensed into Cooper pairs.It should be noted,that also normal conduction is carried by just a small
fraction of the valence electrons,see sect.4.1.
Fig.8:(a) Free energy of aluminium in the normal and superconducting state as a function of T (after N.E.Phillips).The
normal state was achieved by exposing the sample to a ﬁeld larger than H
c
while the superconducting state was measured at
H = 0.(b) Schematic sketch of the free energies G
norm
and G
sup
as a function of the applied ﬁeld B =
0
H.
3.2 Energy balance in a magnetic ﬁeld
We have argued that a lead cylinder becomes superconductive for T < T
c
because the free energy is
reduced that way:
G
sup
< G
norm
for T < T
c
:
What happens if we apply a magnetic ﬁeld?A normalconducting metal cylinder is penetrated by the
ﬁeld so its free energy does not change:G
norm
(H) = G
norm
(0).In contrast to this,a superconducting
cylinder is strongly affected by the ﬁeld.It sets up shielding currents which generate a magnetic moment
~mantiparallel to the applied ﬁeld.The magnetic moment has a positive potential energy in the magnetic
ﬁeld
E
pot
=
0
~m
~
H = +
0
j ~mj j
~
Hj:(6)
In the following it is useful to introduce the magnetisation M as the magnetic moment per unit volume.
The magnetisation of a superconductor inside a currentcarrying coil resembles that of an iron core.The
‘magnetising’ ﬁeld His generated by the coil current only and is unaffected by the presence of a magnetic
material while the magnetic ﬂux density
1
B is given by the superposition of H and the superconductor
magnetisation M:
~
B =
0
(
~
H +
~
M):(7)
In the following I will call both H and B magnetic ﬁelds.For a type I superconductor we have
~
M(
~
H) =
~
H and
~
B = 0 (8)
as long as H < H
c
.The potential energy per unit volume is obtained by integration
E
pot
=
0
Z
H
0
~
M(
~
H
0
)
~
dH
0
=
0
Z
H
0
H
0
2
dH
0
=
0
2
H
2
:(9)
This corresponds to the increase in the Gibbs free energy that is caused by the magnetic ﬁeld,see Fig.
8b.
G
sup
(H) = G
sup
(0) +
0
2
H
2
:(10)
Here and in the following Gdenotes the Gibbs free energy per unit volume.The critical ﬁeld is achieved
when the free energy in the superconducting state just equals the free energy in the normal state
0
2
H
2
c
= G
norm
G
sup
(0):(11)
Since the energy density stored in a magnetic ﬁeld is (
0
=2)H
2
,an alternative interpretation of Eq.(11)
is the following:in order to go from the normal to the superconducting state the material has to push
out the magnetic energy,and the largest amount it can push out is the difference between the two free
energies at vanishing ﬁeld.For H > H
c
the normal phase has a lower energy,so superconductivity
breaks down.
1
There is often a confusion whether the H or the B ﬁeld should be used.Unfortunately,much of the superconductivity
literature is based on the obsolete CGS system of units where the distinction between B and H is not very clear and the two
ﬁelds have the same dimension although their units were given different names:Gauss and Oerstedt.
3.3 Type II superconductors
For practical application in magnets it would be rather unfortunate if only type I superconductors existed
which permit no magnetic ﬁeld and no current in the bulk material.Alloys and the element niobium are
socalled type II superconductors.Their magnetisation curves exhibit a more complicated dependence
on magnetic ﬁeld (Fig.9).Type II conductors are characterized by two critical ﬁelds,H
c1
and H
c2
,
which are both temperature dependent.For ﬁelds 0 < H < H
c1
the substance is in the Meissner phase
with complete exclusion of the ﬁeld fromthe interior.In the range H
c1
< H < H
c2
the substance enters
the mixed phase,often also called Shubnikov phase:part of the magnetic ﬂux penetrates the bulk of the
sample.Above H
c2
,ﬁnally,the material is normalconducting.The area under the curve M = M(H)
is the same as for a type I conductor as it corresponds to the freeenergy difference between the normal
and the superconducting state and is given by (
0
=2) H
2
c
.
Fig.9:Magnetisation of type I and type II superconductors as a function of the magnetic ﬁeld.
It is instructive to compare measured data on pure lead (type I) and leadindium alloys (type II) of
various composition.Figure 10 shows that the upper critical ﬁeld rises with increasing indium content;
for PbIn(20.4%) it is about eight times larger than the critical ﬁeld of pure lead.Under the assumption
that the freeenergy difference is the same for the various leadindium alloys,the areas under the three
curves A,B,C in Fig.10 should be identical as the diagram clearly conﬁrms.
Fig.10:The measured magnetisation curves [14] of leadindium alloys of various composition,plotted against B =
0
H.
A remarkable feature,which will be addressed in more detail later,is the observation that the
magnetic ﬂux does not penetrate the type II conductor with uniform density.Rather it is concentrated in
ﬂux tubes as sketched in Fig.11.Each tube is surrounded with a supervortex current.The material in
between the tubes is ﬁeld and currentfree.
Fig.11:Flux tubes in a type II superconductor.
The fact that alloys stay superconductive up to much higher ﬁelds is easy to understand:magnetic
ﬂux is allowed to penetrate the sample and therefore less magnetic ﬁeld energy has to be driven out.
Figure 12 shows that a type II superconducting cylinder in the mixed phase has a smaller magnetic
moment than a type I cylinder.This implies that the curve G
sup
(H) reaches the level G
sup
(H) = G
norm
at a ﬁeld H
c2
> H
c
.
In a (T;H) plane the three phases of a type II superconductor are separated by the curves H
c1
(T)
and H
c2
(T) which meet at T = T
c
,see Fig.13a.The upper critical ﬁeld can assume very large values
which make these substances extremely interesting for magnet coils (Fig.13b).
Fig.12:Top:Magnetic moment of a type I and a type II sc cylinder in a ﬁeld H
c1
< H < H
c
.Bottom:The Gibbs free
energies of both cylinders as a function of ﬁeld.
Fig.13:(a) The phase diagram of a type II superconductor.(b) The upper critical ﬁeld B
c2
=
0
H
c2
of several highﬁeld
alloys as a function of temperature.
3.4 When is a superconductor of type I or type II?
3.41 Thin sheets of type I superconductors
Let us ﬁrst stick to type I conductors and compare the magnetic properties of a very thin sheet (thickness
d <
L
) to those of a thick slab.The thick slab has a vanishing B ﬁeld in the bulk (Fig.14a) while in the
thin sheet (Fig.14b) the B ﬁeld does not drop to zero at the centre.Consequently less energy needs to be
expelled which implies that the critical ﬁeld of a very thin sheet is much larger than the B
c
of a thick slab.
Fromthis point of viewit might appear energetically favourable for a thick slab to subdivide itself into an
alternating sequence of thin normal and superconducting slices as indicated in Fig.14c.The magnetic
energy is indeed lowered that way but there is another energy to be taken into consideration,namely
the energy required to create the normalsuperconductor interfaces.A subdivision is only sensible if the
interface energy is less than the magnetic energy.
Fig.14:Attenuation of ﬁeld (a) in a thick slab and (b) in thin sheet.(c) Subdivision of a thick slab into alternating layers of
normal and superconducting slices.
3.42 Coherence length
At a normalsuperconductor boundary the density of the supercurrent carriers (the Cooper pairs) does not
jump abruptly from zero to its value in the bulk but rises smoothly over a ﬁnite length ,the coherence
length,see Fig.15.
Fig.15:The exponential drop of the magnetic ﬁeld and the rise of the Cooperpair density at a boundary between a normal and
a superconductor.
The relative size of the London penetration depth and the coherence length decides whether a
material is a type I or a type II superconductor.To study this in a semiquantitative way,we ﬁrst deﬁne
the thermodynamic critical ﬁeld by the energy relation
0
2
H
2
c
= G
norm
G
sup
(0):(12)
For type I this coincides with the known H
c
,see Eq.(11),while for type II conductors H
c
lies between
H
c1
and H
c2
.The difference between the two free energies,G
norm
G
sup
(0),can be intepreted as the
Cooperpair condensation energy.
For a conductor of unit area,exposed to a ﬁeld H = H
c
parallel to the surface,the energy balance
is as follows:
(a) The magnetic ﬁeld penetrates a depth
L
of the sample which corresponds to an energy gain since
magnetic energy must not be driven out of this layer:
E
magn
=
0
2
H
2
c
L
:(13)
(b) On the other hand,the fact that the Cooperpair density does not assume its full value right at the
surface but rises smoothly over a length implies a loss of condensation energy
E
cond
=
0
2
H
2
c
:(14)
Obviously there is a net gain if
L
> .So a subdivision of the superconductor into an alternating
sequence of thin normal and superconducting slices is energetically favourable if the London penetration
depth exceeds the coherence length.
Amore reﬁned treatment is provided by the GinzburgLandau theory [9].Here one introduces the
GinzburgLandau parameter
=
L
=:(15)
The criterion for type I or II superconductivity is found to be
type I: < 1=
p
2
type II: > 1=
p
2.
In reality a type II superconductor is not subdivided into thin slices but the ﬁeld penetrates the
sample in ﬂux tubes which arrange themselves in a triangular pattern.The core of a ﬂux tube is normal.
The following table lists the penetration depths and coherence lengths of some important superconduct
ing elements.Niobium is a type II conductor but close to the border to type I,while indium,lead and tin
are clearly type I conductors.
material
In Pb Sn Nb
L
[nm]
24 32 30 32
[nm]
360 510 170 39
The coherence length is proportional to the mean free path`of the conduction electrons in the metal.
This quantity can be large for a very pure crystal but is strongly reduced by lattice defects and impurity
atoms.In alloys the mean free path is generally much shorter than in pure metals so alloys are always
type II conductors.In the GinzburgLandau theory the upper critical ﬁeld is given by
B
c2
=
p
2 B
c
=
0
2
2
(16)
where
0
is the ﬂux quantum(see sect.5.2).For niobiumtitanium with an upper critical ﬁeld B
c2
= 10
T at 4.2 K this formula yields = 6 nm.The coherence length is larger than the typical width of a grain
boundary in NbTi which means that the supercurrent can move freely from grain to grain.In highT
c
superconductors the coherence length is often shorter than the grain boundary width,and then current
ﬂow from one grain to the next is strongly impeded.There exists no simple expression for the lower
critical ﬁeld.In the limit 1 one gets
B
c1
=
1
2
(ln +0:08)B
c
:(17)
3.5 Heat capacity and heat conductivity
The speciﬁc heat capacity per unit volume at low temperatures is given by the expression
C
V
(T) = T +AT
3
:(18)
The linear term in T comes from the conduction electrons,the cubic term from lattice vibrations.The
coefﬁcients can be calculated within the freeelectrongas model and the Debye theory of lattice speciﬁc
heat (see any standard textbook on solid state physics):
=
2
nk
2
B
2E
F
;A =
12
4
Nk
B
5
3
D
:(19)
Here k
B
= 1:38 10
23
J/K is the Boltzmann constant,E
F
the Fermi energy,n the density of the free
electrons,N the density of the lattice atoms and
D
the Debye temperature of the material.If one plots
the ratio C(T)=T as a function of T
2
a straight line is obtained as can be seen in Fig.16a for normal
conducting gallium[15].In the superconducting state the electronic speciﬁc heat is different because the
electrons bound in Cooper pairs no longer contribute to energy transport.In the BCS theory one expects
an exponential rise of the electronic heat capacity with temperature
C
e;s
(T) = 8:5 T
c
exp(1:44 T
c
=T) (20)
The experimental data (Fig.16a,b) are in good agreement with this prediction.There is a resemblance
to the exponential temperature dependence of the electrical conductivity in intrinsic semiconductors and
these data can be taken as an indication that an energy gap exists also in superconductors.
Fig.16:(a) Speciﬁc heat C(T)=T of normal and superconducting galliumas a function of T
2
[15].(b) Experimental veriﬁca
tion of Eq.(20).
The heat conductivity of niobium is of particular interest for superconducting radio frequency
cavities.Here the theoretical predictions are rather imprecise and measurements are indispensible.The
low temperature values depend strongly on the residual resistivity ratio RRR = R(300 K)=R(10 K) of
the normalconducting niobium.Figure 17 shows experimental data [16].
Fig.17:Measured heat conductivity in niobiumsamples with RRR = 270 and RRR = 500 as a function of temperature [16].
4.BASIC CONCEPTS ANDRESULTS OF THE BCS THEORY
4.1 The ‘free electron gas’ in a normal metal
4.11 The Fermi sphere
In a metal like copper the positively charged ions form a regular crystal lattice.The valence electrons
(one per Cu atom) are not bound to speciﬁc ions but can move through the crystal.In the simplest
quantum theoretical model the Coulomb attraction of the positive ions is represented by a potential well
with a ﬂat bottom,the periodic structure is neglected (taking into account the periodic lattice potential
leads to the electronic band structure of semiconductors).The energy levels are computed by solving the
Schr¨odinger equation with boundary conditions,and then the electrons are placed on these levels paying
attention to the Pauli exclusion principle:no more than two electrons of opposite spin are allowed on
each level.The electrons are treated as independent and noninteracting particles,their mutual Coulomb
repulsion is taken into account only globally by a suitable choice of the depth of the potential well.It
is remarkable that such a simpleminded picture of a ‘free electron gas’ in a metal can indeed reproduce
the main features of electrical and thermal conduction in metals.However,an essential prerequisite is
to apply the FermiDirac statistics,based on the Pauli principle,and to avoid the classical Boltzmann
statistics which one uses for normal gases.The electron gas has indeed rather peculiar properties.The
average kinetic energy of the metal electrons is by no means given by the classical expression
m
e
2
v
2
=
3
2
k
B
T
which amounts to about 0.025 eV at room temperature.Instead,the energy levels are ﬁlled with two
electrons each up to the Fermi energy E
F
.Since the electron density n is very high in metals,E
F
assumes large values,typically 5 eV.The average kinetic energy of an electron is 3=5E
F
3 eV and
thus much larger than the average energy of a usual gas molecule.The electrons constitute a system
called a ‘highly degenerate’ Fermi gas.The Fermi energy is given by the formula
E
F
=
~
2
2m
e
(3
2
n)
2=3
:(21)
Fig.18:The allowed states for conduction electrons in the p
x
p
y
plane and the Fermi sphere.The occupied states are drawn as
full circles,the empty states as open circles.
The quantity ~ = h=2 = 1:05 10
34
Js = 6:58 10
15
eVs is Planck’s constant,the most
important constant in quantum theory.In order to remind the reader I will shortly sketch the derivation
of these results.Consider a threedimensional region in the metal of length L = N a,where a is the
distance of neighbouring ions in the lattice and N 1 an integer.The Schr¨odinger equation with
potential V = 0 and with periodic boundary conditions (x +L;y;z) = (x;y;z) etc.is solved by
(x;y;z) = L
3=2
exp(i(k
1
x +k
2
y +k
3
z)) (22)
where the components of the wave vector
~
k are given by
k
j
= n
j
2
L
with n
j
= 0;1;2;:::(23)
The electron momentum is ~p = ~
~
k,the energy is E = ~
2
~
k
2
=(2m
e
).It is useful to plot the allowed
quantum states of the electrons as dots in momentumspace.In Fig.18 this is drawn for two dimensions.
In the ground state of the metal the energy levels are ﬁlled with two electrons each starting from
the lowest level.The highest energy level reached is called the Fermi E
F
.At temperature T!0 all
states belowE
F
are occupied,all states above E
F
are empty.The highest momentumis called the ‘Fermi
momentum’ p
F
=
p
2m
e
E
F
,the highest velocity is the Fermi velocity v
F
= p
F
=m
e
which is in the
order of 10
6
m/s.In the momentumstate representation,the occupied states are located inside the ‘Fermi
sphere’ of radius p
F
,the empty states are outside.
What are the consequences of the Pauli principle for electrical conduction?Let us apply an electric
ﬁeld
~
E
0
pointing into the negative x direction.In the time t a free electron would gain a momentum
p
x
= eE
0
t:(24)
However,most of the metal electrons are unable to accept this momentum because they do not ﬁnd free
states in their vicinity,only those on the right rimof the Fermi sphere have free states accessible to them
and can accept the additional momentum.We see that the Pauli principle has a strong impact on electrical
conduction.Heat conduction is affected in the same way because the most important carriers of thermal
energy are again the electrons.An anomaly is also observed in the heat capacity of the electron gas.It
differs considerably from that of an atomic normal gas since only the electrons in a shell of thickness
k
B
T near the surface of the Fermi sphere can contribute.Hence the electronic speciﬁc heat per unit
volume is roughly a fraction k
B
T=E
F
of the classical value
C
e
3
2
nk
B
k
B
T
E
F
:
This explains the linear temperature dependence of the electronic speciﬁc heat,see eq.(19).
4.12 The origin of Ohmic resistance
Before trying to understand the vanishing resistance of a superconductor we have to explain ﬁrst why
a normal metal has a resistance.This may appear trivial if one imagines the motion of electrons in a
crystal that is densely ﬁlled with ions.Intuitively one would expect that the electrons can travel for very
short distances only before hitting an ion and thereby loosing the momentumgained in the electric ﬁeld.
Collisions are indeed responsible for a frictional force and one can derive Ohm’s law that way.What is
surprising is the fact that these collisions are so rare.In an ideal crystal lattice there are no collisions
whatsoever.This is impossible to understand in the particle picture,one has to treat the electrons as
matter waves and solve the Schr¨odinger equation for a periodic potential.The resistance is nevertheless
due to collisions but the collision centres are not the ions in the regular crystal lattice but only the
imperfections of this lattice:impurities,lattice defects and the deviations of the metal ions from their
nominal position due to thermal oscillations.The third effect dominates at room temperature and gives
rise to a resistivity that is roughly proportional to T while impurities and lattice defects are responsible
for the residual resistivity at low temperature (T < 20 K).A typical curve (T) is plotted in Fig.19.
In very pure copper crystals the lowtemperature resistivity can become extremely small.The mean free
path of the conduction electrons may be a million times larger than the distance between neighbouring
ions which illustrates very well that the ions in their regular lattice positions do not act as scattering
centres.
Fig.19:Temperature dependence of the resistivity of OFHC (oxygenfree high conductivity) copper and of 99.999% pure
annealed copper.Plotted as a dashed line is the calculated resistivity of copper without any impurities and lattice defects (after
M.N.Wilson [17]).
4.2 Cooper pairs
We consider a metal at T!0.All states inside the Fermi sphere are ﬁlled with electrons while all
states outside are empty.In 1956 Cooper studied [18] what would happen if two electrons were added
to the ﬁlled Fermi sphere with equal but opposite momenta ~p
1
= ~p
2
whose magnitude was slightly
larger than the Fermi momentum p
F
(see Fig.20).Assuming that a weak attractive force existed he was
able to show that the electrons form a bound system with an energy less than twice the Fermi energy,
E
pair
< 2E
F
.The mathematics of Cooper pair formation will be outlined in Appendix B.
Fig.20:A pair of electrons of opposite momenta added to the full Fermi sphere.
What could be the reason for such an attractive force?First of all one has to realize that the
Coulomb repulsion between the two electrons has a very short range as it is shielded by the positive
ions and the other electrons in the metal.So the attractive force must not be strong if the electrons are
several lattice constants apart.Already in 1950,Fr¨ohlich and,independently,Bardeen had suggested
that a dynamical lattice polarization may create a weak attractive potential.Before going into details
let us look at a familiar example of attraction caused by the deformation of a medium:a metal ball is
placed on an elastic membrane and deforms the membrane such that a potential well is created.Asecond
ball will feel this potential well and will be attracted by it.So effectively,the deformation of the elastic
membrane causes an attractive force between the two balls which would otherwise not notice each other.
This visualisation of a Cooperpair is well known in the superconductivity community (see e.g.[1]) but
it has the disadvantage that it is a static picture.
I prefer the following dynamic picture:suppose you are crosscountry skiing in very deep snow.
You will ﬁnd this quite cumbersome,there is a lot of ‘resistance’.Now you discover a track made by
another skier,a ‘Loipe’,and you will immediately realize that it is much more comfortable to ski along
this track than in any other direction.The Loipe picture can be adopted for our electrons.The ﬁrst
electron ﬂies through the lattice and attracts the positive ions.Because of their inertia they cannot follow
immediately,the shortest response time corresponds to the highest possible lattice vibration frequency.
This is called the Debye frequency!
D
.The maximum lattice deformation lags behind the electron by a
distance
d v
F
2
!
D
100 1000 nm:(25)
Fig.21:Dynamical deformation of the crystal lattice caused by the passage of a fast electron.(After Ibach,L¨uth [19]).
Obviously,the lattice deformation attracts the second electron because there is an accumulation of
positive charge.The attraction is strongest when the second electron moves right along the track of the
ﬁrst one and when it is a distance d behind it,see Fig.21.This explains why a Cooper pair is a very
extended object,the two electrons may be several 100 to 1000 lattice constants apart.For a simple cubic
lattice,the lattice constant is the distance between adjacent atoms.
In the example of the crosscountry skiers or the electrons in the crystal lattice,intuition suggests
that the second partner should preferably have the same momentum,~p
2
= ~p
1
although opposite momenta
~p
2
= ~p
1
are not so bad either.Quantum theory makes a unique choice:only electrons of opposite
momenta form a bound system,a Cooper pair.I don’t know of any intuitive argument why this is so.
(The quantum theoretical reason is the Pauli principle but there exists probably no intuitive argument
why electrons obey the Pauli exclusion principle and are thus extreme individualists while other particles
like the photons in a laser or the atoms in superﬂuid helium do just the opposite and behave as extreme
conformists.One may get used to quantumtheory but certain mysteries and strange feelings will remain.)
The binding energy of a Cooper pair turns out to be small,10
4
10
3
eV,so lowtemperatures are
needed to preserve the binding in spite of the thermal motion.According to Heisenberg’s Uncertainty
Principle a weak binding is equivalent to a large extension of the composite system,in this case the
abovementioned d = 100 1000 nm.As a consequence,the Cooper pairs in a superconductor overlap
each other.In the space occupied by a Cooper pair there are about a million other Cooper pairs.Figure
22 gives an illustration.The situation is totally different fromother composite systems like atomic nuclei
or atoms which are tightly bound objects and wellseparated from another.The strong overlap is an
important prerequisite of the BCS theory because the Cooper pairs must change their partners frequently
in order to provide a continuous binding.
Fig.22:Visualization of Cooper pairs and single electrons in the crystal lattice of a superconductor.(After Essmann and
Tr¨auble [12]).
4.3 Elements of the BCS theory
After Cooper had proved that two electrons added to the ﬁlled Fermi sphere are able to form a bound
system with an energy E
pair
< 2E
F
,it was immediately realized by Bardeen,Cooper and Schrieffer
that also the electrons inside the Fermi sphere should be able to group themselves into pairs and thereby
reduce their energy.The attractive force is provided by lattice vibrations whose quanta are the phonons.
The highest possible phonon energy is
~!
D
= k
B
D
0:01 0:02 eV:(26)
Therefore only a small fraction of the electrons can be paired via phonon exchange,namely those in
a shell of thickness ~!
D
around the Fermi energy.This is sketched in Fig.23.The inner electrons
cannot participate in the pairing because the energy transfer by the lattice is too small.One has to keep
in mind though that these electrons do not contribute to normal conduction either.For vanishing electric
ﬁeld a Cooper pair is a loosely bound system of two electrons whose momenta are of equal magnitude
but opposite direction.All Cooper pairs have therefore the same momentum
~
P = 0 and occupy exactly
the same quantum state.They can be described by a macroscopic wave function in analogy with the
light wave in a laser in which the photons are all in phase and have the same wavelength,direction and
polarisation.The macroscopic photon wave function is the vector potential from which one can derive
the electric and magnetic ﬁeld vectors (see sect.5.2).
Fig.23:Various Cooper pairs (~p;~p);(~p
0
;~p
0
);(~p
00
;~p
00
);:::in momentum space.
The reason why Cooper pairs are allowed and even prefer to enter the same quantum state is that
they behave as Bose particles with spin 0.This is no contradiction to the fact that their constituents are
spin 1/2 Fermi particles.Figure 23 shows very clearly that the individual electrons forming the Cooper
pairs have different momentumvectors ~p;~p
0
;~p
00
;:::which however cancel pairwise such that the pairs
have all the same momentumzero.It should be noted,though,that Cooper pairs differ considerably from
other Bosons such as helium nuclei or atoms:They are not ‘small’ but very extended objects,they exist
only in the BCS ground state and there is no excited state.An excitation is equivalent to breaking them
up into single electrons.
The BCS ground state is characterized by the macroscopic wave function and a ground state
energy that is separated from the energy levels of the unpaired electrons by an energy gap.In order to
break up a pair an energy of 2is needed,see Fig.24.
Fig.24:(a) Energy gap between the BCS ground state and the singleelectron states.(b) Reduction of energy gap in case of
current ﬂow.
There is a certain similarity with the energy gap between the valence band and the conduction
band in a semiconductor but one important difference is that the energy gap in a superconductor is not
a constant but depends on temperature.For T!T
c
one gets (T)!0.The BCS theory makes
a quantitative prediction for the function (T) which is plotted in Fig.25 and agrees very well with
experimental data.
Fig.25:Temperature dependence of the energy gap according to the BCS theory and comparison with experimental data.
One of the fundamental formulae of the BCS theory is the relation between the energy gap (0)
at T = 0,the Debye frequency!
D
and the electronlattice interaction potential V
0
:
(0) = 2~!
D
exp
1
V
0
N(E
F
)
:(27)
Here N(E
F
) is the density of singleelectron states of a given spin orientation at E = E
F
(the other spin
orientation is not counted because a Cooper pair consists of two electrons with opposite spin).Although
the interaction potential V
0
is assumed to be weak,one of the most striking observations is that the
exponential function cannot be expanded in a Taylor series around V
0
= 0 because all coefﬁcients vanish
identically.This implies that Eq.(27) is a truely nonperturbative result.The fact that superconductivity
cannot be derived from normal conductivity by introducing a ‘small’ interaction potential and applying
perturbation theory (which is the usual method for treating problems of atomic,nuclear and solid state
physics that have no analytical solution) explains why it took so many decades to ﬁnd the correct theory.
The critical temperature is given by a similar expression
k
B
T
c
= 1:14 ~!
D
exp
1
V
0
N(E
F
)
:(28)
Combining the two equations we arrive at a relation between the energy gap and the critical temperature
which does not contain the unknown interaction potential
(0) = 1:76 k
B
T
c
:(29)
The following table shows that this remarkable prediction is fulﬁlled rather well.
element
Sn In Tl Ta Nb Hg Pb
(0)=k
B
T
c
1:75 1:8 1:8 1:75 1:75 2:3 2:15
In the BCS theory the underlying mechanism of superconductivity is the attractive force between
pairs of electrons that is provided by lattice vibrations.It is of course highly desirable to ﬁnd experimental
support of this basic hypothesis.According to Eq.(28) the critical temperature is proportional to the
Debye frequency which in turn is inversely proportional to the square root of the atomic mass M:
T
c
/!
D
/1=
p
M:
If one produces samples fromdifferent isotopes of a superconducting element one can check this relation.
Figure 26 shows T
c
measurements on tin isotopes.The predicted 1=
p
M law is very well obeyed.
Fig.26:The critical temperature of various tin isotopes.
4.4 Supercurrent and critical current
The most important task of a theory of superconductivity is of course to explain the vanishing resistance.
We have seen in sect.4.1 that the electrical resistance in normal metals is caused by scattering processes
so the question is why Cooper pairs do not suffer from scattering while unpaired electrons do.To start
a current in the superconductor,let us apply an electric ﬁeld
~
E
0
for a short time t.Both electrons of a
Cooper pair receive an additional momentum ~p = e
~
E
0
t so after the action of the ﬁeld all Cooper
pairs have the same nonvanishing momentum
~
P = ~
~
K = 2
~
E
0
t:
Associated with this coherent motion of the Cooper pairs is a supercurrent density
~
J
s
= n
c
e~
m
e
~
K:(30)
Here n
c
is the Cooperpair density.It can be shown (see e.g.Ibach,L¨uth [19]) that the Cooperpair
wave function with a current ﬂowing is simply obtained by multiplying the wave function at rest with
the phase factor exp(i
~
K
~
R) where
~
R = (~r
1
+~r
2
)=2 is the coordinate of the centre of gravity of the
two electrons.Moreover the electronlattice interaction potential is not modiﬁed by the current ﬂow.
So all equations of the BCS theory remain applicable and there will remain an energy gap provided the
kineticenergy gain E
pair
of the Cooper pair is less than 2,see Fig.24b.It is this remaining energy
gap which prevents scattering.As we have seen there are two types of scattering centres:impurities
and thermal lattice vibrations.Cooper pairs can only scatter when they gain sufﬁcient energy to cross the
energy gap and are then broken up into single electrons.An impurity is a ﬁxed heavy target and scattering
cannot increase the energy of the electrons of the pair,therefore impurity scattering is prohibited for the
Cooper pairs.Scattering on thermal lattice vibrations is negligible as long as the average thermal energy
is smaller than the energy gap (that means as long as the temperature is less than the critical temperature
for the given current density).So we arrive at the conclusion that there is resistancefree current transport
provided there is still an energy gap present (2E
pair
> 0) and the temperature is sufﬁciently low
(T < T
c
(J
s
)).
The supercurrent density is limited by the condition that the energy gain E
pair
must be less than
the energy gap.This leads to the concept of the critical current density J
c
.The energy of the Cooper
pair is,after application of the electric ﬁeld,
E
pair
=
1
2m
e
(~p +
~
P=2)
2
+(~p +
~
P=2)
2
=
~p
2
m
e
+E
pair
with E
pair
p
F
P=m
e
.Fromthe condition E
pair
2we get
J
s
J
c
2e n
c
=p
F
:(31)
Coupled to a maximum value of the current density is the existence of a critical magnetic ﬁeld.The
current ﬂowing in a long wire of type I superconductor is conﬁned to a surface layer of thickness
L
,see
Fig.6c.The maximumpermissible current density J
c
is related to the critical ﬁeld:
H
c
(T) =
L
J
c
(T)
L
2en
c
(T)=p
F
:(32)
The temperature dependence of the critical ﬁeld is caused by the temperature dependence of the gap
energy.
The above considerations on resistancefree current ﬂow may appear a bit formal so I would like
to give a more familiar example where an energy gap prevents ‘resistance’ in a generalized sense.We
compare crystals of diamond and silicon.Diamond is transparent to visible light,silicon is not.So silicon
represents a ‘resistance’ to light.Why is this so?Both substances have exactly the same crystal structure,
namely the ‘diamond lattice’ that is composed of two facecentred cubic lattices which are displaced by
one quarter along the spatial diagonal.The difference is that diamond is built up fromcarbon atoms and
is an electrical insulator while a silicon crystal is a semiconductor.In the band theory of solids there
is an energy gap E
g
between the valence band and the conduction band.The gap energy is around 7
eV for diamond and 1 eV for silicon.Visible light has a quantum energy of about 2.5 eV.A photon
impinging on a silicon crystal can lift an electron from the valence band to the conduction band and is
thereby absorbed.The same photon impinging on diamond is unable to supply the required energy of 7
eV,so this photon simply passes the crystal without absorption:diamond has no ‘resistance’ for light.
(Quantum conditions of this kind have already been known in the Stone Age.If hunters wanted to catch
an antelope that could jump 2 m high,they would dig a hole 4 m deep and then the animal could never
get out because being able to jump 2 min two successive attempts is useless for overcoming the 4 m.The
essential feature of a quantum process,namely that the energy gap has to be bridged in a single event,is
already apparent in this trivial example).
Finally,I want to give an example for frictionless current ﬂow.The hexagonal benzene molecule
C
6
H
6
is formed by covalent binding and contains 24 electrons which are localised in bonds in the
plane of the molecule and 6 electrons in bonds below and above this plane.The electrons can
move freely around the ring.By a timevarying magnetic ﬁeld a ring current is induced (benzene is
a diamagnetic molecule) which will run forever unless the magnetic ﬁeld is changed.This resembles
closely the operation of a superconducting ring in the persistent mode (see Fig.27).
Fig.27:Persistent ring currents in a benzene molecule and in a superconducting ring which have been induced by a rising ﬁeld
B
z
.
5.QUANTISATIONOF MAGNETICFLUX
Several important superconductor properties,in particular the magnetic ﬂux quantisation,can only be
explained by studying the magnetic vector potential and its impact on the socalled ‘canonical momen
tum’ of the charge carriers.Since this may not be a familiar concept I will spend some time to discuss
the basic ideas and the supporting experiments which are beautiful examples of quantum interference
phenomena.
5.1 The vector potential in electrodynamics
In classical electrodynamics it is often a matter of convenience to express the magnetic ﬁeld as the curl
(rotation) of a vector potential
~
B =
~
r
~
A:
The magnetic ﬂux through an area F can be computed from the line integral of
~
A along the rimof F by
using Stoke’s theorem:
mag
=
Z Z
~
B
~
dF =
I
~
A
~
ds:(33)
We apply this to the solenoidal coil sketched in Fig.28.
Fig.28:Magnetic ﬁeld and vector potential of a solenoid.
The magnetic ﬁeld has a constant value B = B
0
inside the solenoid and vanishes outside if we the
length of the coil is much larger than its radius R.The vector potential has only an azimuthal component
and can be computed using Eq.(33):
A
(r) =
8
<
:
1
2
B
0
r for r < R
1
2
B
0
R
2
r
for r > R:
Evaluating
~
B =
~
r
~
A in cylindrical coordinates gives the expected result
B
z
(r) =
B
0
for r < R
0 for r > R:
What do we learn from this example?
(a) The vector potential is parallel to the current but perpendicular to the magnetic ﬁeld.
(b) There are regions in space where the vector potential is nonzero while the magnetic ﬁeld vanishes.
Here it is the region r > R.A circular contour of radius r > R includes magnetic ﬂux,namely B
0
R
2
for all r > R,so
~
A must be nonzero,although
~
B = 0.
The vector potential is not uniquely deﬁned.A new potential
~
A
0
=
~
A +
~
r with an arbitrary
scalar function (x;y;z) leaves the magnetic ﬁeld
~
B invariant because the curl of a gradient vanishes
identically.For this reason it is often said that the vector potential is just a useful mathematical quantity
without physical signiﬁcance of its own.In quantum theory this point of view is entirely wrong,the
vector potential is of much deeper physical relevance than the magnetic ﬁeld.
5.2 The vector potential in quantumtheory
In quantum theory the vector potential is a quantity of fundamental importance:
(1)
~
A is the wave function of the photons,
(2) in an electromagnetic ﬁeld the wavelength of a charged particle is modiﬁed by the vector potential.
For the application in superconductivity we are interested in the second aspect.The de Broglie relation
states that the wavelength we have to attribute to a particle is Planck’s constant divided by the particle
momentum
=
2~
p
:(34)
For a free particle one has to insert p = mv.It turns out that in the presence of an electromagnetic
ﬁeld this is no longer correct,instead one has to replace the mechanical momentum m~v by the socalled
‘canonical momentum’
~p = m~v +q
~
A (35)
where q is the charge of the particle (q = e for an electron).The wavelength is then
=
2~
mv +qA
:
If one moves by a distance x,the phase'of the electron wave function changes in free space by the
amount
'=
2
x =
1
~
m
e
~v
~
x:
In an electromagnetic ﬁeld there is an additional phase change
'
0
=
e
~
~
A
~
x:
This is called the AharonovBohm effect after the theoreticians who predicted the phenomenon [20].The
phase shift should be observable in a doubleslit experiment as sketched in Fig.29.An electron beam is
split into two coherent subbeams and a tiny solenoid coil is placed between these beams.The subbeam
1 travels antiparallel to
~
A,beam 2 parallel to
~
A.So the two subbeams gain a phase difference
'= '
0
+
e
~
I
~
A
~
ds = '
0
+
e
~
mag
:(36)
Fig.29:Schematic arrangement for observing the phase shift due to a vector potential.
Here '
0
is the phase difference for current 0 in the coil.The AharonovBohm effect was veriﬁed
in a beautiful experiment by M¨ollenstedt and Bayh in T¨ubingen [21].The experimental setup and the
result of the measurements are shown in Fig.30.An electron beam is split by a metalized quartz
ﬁbre on negative potential which acts like an optical biprism.Two more ﬁbres bring the two beams
to interference on a photographic ﬁlm.Very sharp interference fringes are observed.Between the sub
beams is a 14 m–diameter coil wound from 4 m thick tungsten wire.The current in this coil is ﬁrst
zero,then increased linearly with time and after that kept constant.The ﬁlm recording the interference
pattern is moved in the vertical direction.Thereby the moving fringes are depicted as inclined lines.The
observed shifts are in quantitative agreement with the prediction of Eq.(36).
Fig.30:Sketch of the M¨ollenstedtBayh experiment and observed interference pattern.
An interesting special case is the phase shift '= that interchanges bright and dark fringes.
According to Eq.(36) this requires a magnetic ﬂux
mag
=
~
e
=
h
2e
which turns out to be identical to the elementary ﬂux quantum in superconductors,see sect.5.3.In
the M¨ollenstedt experiment however,continuous phase shifts much smaller than are visible,so the
magnetic ﬂux through the normalconducting tungsten coil is not quantised (there is also no theoretical
reason for ﬂux quantisation in normal conductors).
Although the magnetic ﬁeld is very small outside the solenoid,and the observed phase shifts are in
quantitative agreement with the expectation based on the vector potential,there have nevertheless been
sceptics who tried to attribute the observed effects to some stray magnetic ﬁeld.To exclude any such
explanation a newversion of the experiment has recently been carried out by Tonomura et al.[22] making
use of electron holography (Fig.31).A parallel electron beamis imaged by an electron microscope lens
on a photographic plate.To create a holographic pattern the object is placed in the upper half of the
beam while the lower half serves as a reference beam.A metalized quartz ﬁbre (the biprism) brings the
twopart beam to an overlap on the plate.The magnetic ﬁeld is provided by a permanently magnetised
ring of with a few m diameter.The magnet is enclosed in niobium and cooled by liquid helium so the
magnetic ﬁeld is totally conﬁned.The vector potential,however,is not shielded by the superconductor.
The ﬁeld lines of
~
B and
~
A are also drawn in the ﬁgure.The holographic image shows again a very
clear interference pattern and a shift of the dark line in the opening of the ring which is caused by the
vector potential.This experiment demonstrates beyond any doubt that it is the vector potential and not
the magnetic ﬁeld which inﬂuences the wavelength of the electron and the interference pattern.
Fig.31:Observation of AharonovBohm effect using electron holography (after Tonomura [22]).The permanent toroidal
magnet,encapsuled in superconducting niobium,and the observed interference fringes are shown.
5.3 Flux quantisation
The MeissnerOchsenfeld effect excludes magnetic ﬁeld from the bulk of a type I superconductor.An
interesting situation arises if one exposes a superconducting ring to a magnetic ﬁeld.Then one can
obtain a trapped ﬂux,threading the hole of the ring as shown in Fig.32.Both the London and the BCS
theory make the surprising prediction that the ﬂux through the hole cannot assume arbitrary values but is
quantised,i.e.that it is an integer multiple of an elementary ﬂux quantum
mag
= n
0
;n = 0;1;2;:::(37)
Fig.32:Trapping of magnetic ﬂux in a ring.First the normalconducting ring (T > T
c
) is placed in a magnetic ﬁeld,then it is
cooled down (a) and ﬁnally the ﬁeld is switched off (b).The integration path is shown in part (c).
The ﬂux quantumis Planck’s constant divided by the charge of the supercurrent carriers.The BCS
ﬂux quantum is thus
0
=
h
2e
(38)
while the London ﬂux quantumis twice as big because the charge carriers in the London theory are single
electrons.
5.31 Derivation of ﬂux quantisation
The Cooperpair wave function in the ring can be written as
=
p
n
c
exp(i'):
The density of Cooper pairs is denoted as n
c
.The phase'='(s) has to change by n 2 when going
once around the ring since must be a singlevalued wave function.We choose a circular path in the
bulk of the ring (Fig.31c).Then
I
d'
ds
ds = n 2:
In other words:the circumference must be an integer number of wavelengths.In the bulk there is no
current allowed so the Cooperpair velocity must be zero,~v = 0.Therefore the integrand is
d'
ds
ds =
q
~
~
A
~
ds:
Using Eq.(33) we see that the magnetic ﬂux enclosed by the circular path is
mag
=
I
~
A
~
ds =
~
q
n 2 = n
0
)
0
=
2~
q
:(39)
In the BCS theory we have q = 2e and hence
0
= h=(2e).
5.32 Experimental veriﬁcation of ﬂux quantisation
In 1961 two experiments on ﬂux quantisation were carried out almost simultaneously,by Doll and
N¨abauer [23] in M¨unchen and by Deaver and Fairbank [24] in Stanford.I describe the DollN¨abauer
experiment as it yielded the best evidence.The setup and the results are shown in Fig.33.The supercon
ducting ring is here a lead tube prepared by evaporation of lead on a 10 m–thick quartz cylinder which
is then suspended by a torsion ﬁbre.Magnetic ﬂux is captured in the tube by exposing the warmtube to a
‘magnetising ﬁeld’ B
mag
parallel to the axis,cooling down and switching off the ﬁeld.Then a transverse
oscillating ﬁeld B
osc
is applied to induce forced oscillations which are observed by light reﬂection froma
small mirror.The resonant amplitude A
res
is proportional to the magnetic moment of the tube and hence
to the captured magnetic ﬂux.Without ﬂux quantisation the relation between resonant amplitude and
magnetising ﬁeld should be linear.Instead one observes a very pronounced staircase structure which
can be uniquely related to frozenin ﬂuxes of 0,1 or 2 ﬂux quanta.Both experiments proved that the
magnetic ﬂux quantumis h=2e and not h=e and thus gave strong support for the Cooperpair hypothesis.
Fig.33:Observation of ﬂux quantisation [23].
The BCS theory is not directly applicable to highT
c
superconductors
2
which are basically two
dimensional superconductors.In Fig.34 the ﬂux through a YBa
2
Cu
3
O
7
ring with a weak joint is shown.
Flux jumps due to external ﬁeld variations occur in multiples of h=2e which is an indication that some
kind of Cooper pairing is also responsible for the superconductivity in these materials.
Fig.34:Flux through an YBa
2
Cu
3
O
7
ring with a weak link [26].
In another interesting experiment a lead strip was bent into ring shape and closed via an interme
diate YBa
2
Cu
3
O
7
piece.It was possible to induce a persistent ring current in this combined system of a
lowT
c
and a highT
c
superconductor.
5.4 Fluxoid pattern in type II superconductors
Abrikosov predicted that a magnetic ﬁeld penetrates a type II superconductor in the form of ﬂux tubes
or ﬂuxoids,each containing a single elementary quantum
0
,which arrange themselves in a quadratic
or triangular pattern to minimize the potential energy related to the mutual repulsion of the ﬂux tubes.A
schematic cross section of a ﬂuxoid is presented in Fig.35.The magnetic ﬁeld lines are surrounded by
2
For a review of highTc superconductors see ref.[25] and the lectures by R.Fluekiger.
a supercurrent vortex.The Cooperpair density drops to zero at the centre of the vortex,so the core of a
ﬂux tube is normalconducting.
Fig.35:Schematic cross section of a ﬂuxoid.
Fig.36:(a) Fluxoid pattern in niobium(courtesy U.Essmann).The distance between adjacent ﬂux tubes is 0.2 m.(b) Fluxoid
motion in a currentcarrying type II superconductor.
The area occupied by a ﬂuxoid is roughly given by
2
where is the coherence length.An estimate of
the upper critical ﬁeld is derived from the condition that the ﬂuxoids start touching each other:
B
c2
0
2
2
:(40)
An important experimental step was the direct observation of the ﬂuxoid pattern.Essmann and
Tr¨auble [12] developed a ‘decoration’ technique for this purpose.A superconductor sample was cooled
by a liquid helium bath with the surface sticking out of the liquid.Iron was evaporated at some distance
from the superconductor,and in the helium gas atmosphere the iron atoms agglomerated to tiny crystals
(about 20 nm) that were attracted by the magnetic ﬁeld lines and stuck to the sample surface where the
ﬂuxoids emerged.After warming up,a thin ﬁlmwas sprayed on the surface to allowthe iron crystals to be
removed for subsequent observation in an electron microscope.The photograph in Fig.36a shows indeed
the perfect triangular pattern predicted by Abrikosov.Similar pictures have been recently obtained with
hightemperature superconductors.The electron holography setup mentioned in the last section permits
direct visualization of the magnetic ﬂux lines.Figure 37 is an impressive example of the capabilities of
this advanced method.
Fig.37:Holographic image of the magnetic ﬂux lines through a thin lead plate [22].
6.Hard Superconductors
6.1 Flux ﬂow resistance and ﬂux pinning
For application in accelerator magnets a superconducting wire must be able to carry a large current in
the presence of a ﬁeld in the 5 – 10 Tesla range.Type I superconductors are deﬁnitely ruled out because
their critical ﬁeld is less than a few tenths of a Tesla and their currentcarrying capacity is very small
since the current is restricted to a thin surface layer (compare Fig.6).Type II conductors appear quite
appropriate on ﬁrst sight:they have a large upper critical ﬁeld and high currents are permitted to ﬂow in
the bulk material.Still there is a problem,called ﬂux ﬂow resistance.If a current ﬂows through an ideal
type II superconductor which is exposed to a magnetic ﬁeld one observes heat generation.The current
density
~
J exerts a Lorentz force on the ﬂux lines.The force per unit volume is
~
F =
~
J
~
B:
The ﬂux lines begin to move through the specimen in a direction perpendicular to the current and to
the ﬁeld (Fig.36b).This is a viscous motion (~v/
~
F) and leads to heat generation.So although the
current itself ﬂows without dissipation the sample acts as if it had an Ohmic resistance.The statement
is even formally correct.The moving ﬂuxoids represent a moving magnetic ﬁeld.According to Special
Relativity this is equivalent to an electric ﬁeld
~
E
equiv
=
1
c
2
~
B ~v:
It is easy to see that
~
E
equiv
and
~
J point in the same direction just like in a normal resistor.Flux ﬂow
resistance was studied experimentally by Kimand coworkers [28].
To obtain useful wires for magnet coils the ﬂux motion has to be inhibited.The standard method is
to capture them at pinning centres.The most important pinning centres in niobiumtitanium are normal
conducting Ti precipitates with a size in the 10 nm range.Flux pinning is discussed in detail in M.N.
Wilson’s lectures at this school.A type II superconductor with strong pinning is called a hard super
conductor.Hard superconductors are very well suited for highﬁeld magnets,they permit dissipationless
current ﬂow in high magnetic ﬁelds.There is a penalty,however:these conductors exhibit a strong
magnetic hysteresis which is the origin of the very annoying ‘persistentcurrent’ multipoles in supercon
ducting accelerator magnets.
6.2 Magnetisation of a hard superconductor
A type I superconductor shows a reversible response
3
to a varying external magnetic ﬁeld H.The
magnetization is given by the linear relation
~
M(
~
H) =
~
H for 0 < H < H
c
and then drops to zero,
see Fig.10.An ideal type II conductor without any ﬂux pinning should also react reversibly.A hard
superconductor,on the other hand,is only reversible in the Meissner phase because then no magnetic
ﬁeld enters the bulk,so no ﬂux pinning can happen.If the ﬁeld is raised beyond H
c1
magnetic ﬂux enters
the sample and is captured at pinning centres.When the ﬁeld is reduced again these ﬂux lines remain
bound and the specimen keeps a frozenin magnetisation even for vanishing external ﬁeld.One has to
invert the ﬁeld polarity to achieve M = 0 but the initial state (H = 0 and no captured ﬂux in the bulk
material) can only be recovered by warming up the specimen to destroy superconductivity and release
all pinned ﬂux quanta,and by cooling down again.
A typical hysteresis curve is shown in Fig.38a.There is a close resemblence with the hysteresis
in iron except for the sign:the magnetisation in a superconductor is opposed to the magnetising ﬁeld be
cause the underlying physical process is diamagnetism.In an accelerator the ﬁeld is usually not inverted
and then the hysteresis has the shape plotted in Fig.38b.
Fig.38:(a) Magnetic hysteresis of a hard superconductor.(b) Magnetisation hysteresis for the ﬁeld cycle of accelerator
magnets.
Detailed studies on superconductor magnetisation were performed in the HERA dipoles.The
sextupole component is a good measure of M.Immediately after cooldown a dipole was excited to
low ﬁelds.In Fig.39 the sextupole ﬁeld B
3
at a distance of 25 mm from the dipole axis is plotted as
a function of the dipole ﬁeld B
1
=
0
H
1
on the axis.One can see that the sextupole is a reversible
function of B
1
up to about 25 mT (the lower critical ﬁeld of NbTi is somewhat smaller,around 15 mT,
but in most parts of the coil the local ﬁeld is less than the value B
1
on the axis).The superconducting
cable is therefore in the Meissner phase.Increasing B
1
to 50 mT already leads to a slight hysteresis so a
certain amount of magnetic ﬂux enters the NbTi ﬁlaments and is captured there.
3
This statement applies only for long cylindral or elliptical samples oriented parallel to the ﬁeld.
Fig.39:Sextupole ﬁeld in a HERA dipole in the Meissner phase and slightly above.
With increasing ﬁeld the hysteresis widens more and more and is eventually nearly symmetric to
the horizontal axis.The sextupole hysteresis observed in the standard ﬁeld cycle at HERA is plotted in
Fig.40a.A similar curve is obtained for the 12pole in the quadrupoles.
Fig.40:(a) The sextupole component in the HERA dipoles for the standard ﬁeld cycle 4.7 T!0.05 T!4.7 T.(b) Sextupole
ﬁeld for the ﬁrst beam test with positrons of 7 GeV.
Only in a ‘virgin’ magnet,that is right after cooldown,is there the chance to inﬂuence the width
of the hysteresis curve.This fact was used to advantage during the commissioning of the HERA proton
storage ring.The ﬁrst beam test was made with positrons of only 7 GeV since the nominal 40 GeV
protons were not yet available.At the corresponding dipole ﬁeld of 70 mT (coil current 42.5 A) the
persistentcurrent sextupole component would have been two orders of magnitude larger than tolerable
if the standard ﬁeld cycle had been used.To eliminate the sextupole,all magnets were warmed to 20
K to extinguish any previous superconductor magnetisation and cooled back to 4.4 K.Then the current
loop 0!112 A!42.5 A was performed which resulted in an almost vanishing sextupole (see Fig.
40b).A similar procedure was used in the ﬁrst run with 40 GeV protons,this time with the loop 0!
314 A!245 A.The measured chromaticity indeed proved an almost perfect sextupole cancellation.
For the routine operation of HERA these procedures are of course not applicable because they require a
warmup of the whole ring.Instead,sextupole correction coils must be used to compensate the unwanted
ﬁeld distortions.
6.3 Flux creep
The pinning centres prevent ﬂux ﬂow in hard superconductors but some small ﬂux creep effects remain.
At ﬁnite temperatures,even as low as 4 K,a few of the ﬂux quanta may be released from their pinning
locations by thermal energy and then move out of the specimen thereby reducing the magnetisation.The
ﬁrst ﬂux creep experiment was carried out by Kim et al.[29] using a small NbZr tube.If one plots the
internal ﬁeld at the centre of the tube as a function of the external ﬁeld the wellknown hysteresis curve
is obtained in which one can distinguish the shielding and the trapping branch,see Fig.41a.Kim and
coworkers realized that on the trapping branch the internal ﬁeld exhibited a slow logarithmic decrease
with time while on the shielding branch a similar increase was seen (Fig.41b).
Fig.41:(a) Hysteresis of the internal ﬁeld in a tube of hard superconductor.(b) Time dependence of the internal ﬁeld on the
trapping and the shielding branch [29].
A logarithmic time dependence is something rather unusual.In an electrical circuit with inductive
and resistive components the current decays exponentially like exp(t=) with a time constant =
L=R.A theoretical model for thermally activated ﬂux creep was proposed by Anderson [30].The
pinning centres are represented by potential wells of average depth U
0
and width a in which bundles of
ﬂux quanta with an average ﬂux
av
= n
0
are captured.At zero current the probability that ﬂux leaves
a potential well is proportional to the Boltzmann factor
P
0
/exp(U
0
=k
B
T):
When the superconductor carries a current density J the potential acquires a slope proportional to the
force density F/
av
J.This slope reduces the effective potential well depth to U = U
0
Uwith
U
av
Jal,see Fig.42.Here l is the length of the ﬂux bundle.The probability for ﬂux escape
increases
P = P
0
exp(+U=k
B
T):
Fig.42:Sketch of the pinning potential without and with current ﬂow and ﬁeld proﬁle across the NbZr tube.
We consider now the tube in the Kim experiment at a high external ﬁeld B
ext
on the trapping
branch of the hysteresis curve.The internal ﬁeld is then slightly larger,namely by the amount B
int
B
mext
=
0
J
c
w where J
c
is the critical current density at the given temperature and magnetic ﬁeld
and w the wall thickness.Under the assumption B
int
B
ext
B
ext
both ﬁeld and current density are
almost constant throughout the wall.The reduction in well depth U is proportional to the product of
these quantities.If a bundle of ﬂux quanta is released from its well,it will ‘slide’ down the slope and
leave the material.In this way space is created for some magnetic ﬂux from the bore of the cylinder
which will migrate into the conductor and reﬁll the well.As a consequence the internal ﬁeld decreases
and with it the critical current density in the wall.Its time derivative is roughly given by the expression
dJ
c
dt
C exp
U
k
B
T
C exp
av
aJ
c
l
k
B
T
(41)
where C is a constant.The solution of this unusual differential equation is
J
c
(t) = J
c
(0)
k
B
T
av
al
lnt:(42)
This result implies that for given temperature and magnetic ﬁeld the critical current density is not really
a constant but depends slightly on time.What one usually quotes as J
c
is the value obtained after the
decay rate on a linear time scale has become unmeasurably small.
Anearly logarithmic time dependence is also observed in the persistentcurrent multipole ﬁelds of
accelerator magnets,see e.g.[31].So it seems tempting to attribute the effect to ﬂux creep.Surprisingly,
the decay rates are generally much larger than typical ﬂux creep rates and depend moreover on the
maximumﬁeld level in a preceding excitation,see Fig.43a.
Fig.43:(a) Decay of the sextupole coefﬁcient in a HERA dipole at a ﬁeld of 0.23 T for different values of the maximum ﬁeld
in the initialising cycle 0!B
max
!0:04T!0.23 T [32].(b) Magnetisation decay at zero ﬁeld in a long sample of HERA
cable for different values of the maximum ﬁeld in the initialising cycle 0!B
max
!0 [33].
In cable samples this is not the case as is evident from Fig.43b.The average magnetisation of a 5
mlong cable sample decays at lowﬁeld (B = 0 in this case) by less than 1%per decade of time,and the
decay rate is totally independent of the maximum ﬁeld B
max
in the preceding cycle.The observed rate
agrees well with other data on ﬂux creep in NbTi.
From the data in Fig.43 it is obvious that thermally activated ﬂux creep can explain only part of
the time dependence of multipoles in magnets.The decay rates measured in magnets are usually much
larger than those in cable samples,and there is a considerable variation frommagnet to magnet.In 1995
experimental results [34] and model calculations [35] were presented showing that the time dependence
is due to a complex interplay between magnetisation currents in the NbTi ﬁlaments and eddy currents
among the strands of the cable.Quantitative predictions are not possible because of too many unknown
parameters.For a more detailed discussion see [31].
Flux creep has become an important issue after the discovery of hightemperature superconduc
tors.Figure 44 shows that the magnetisation of YBaCuOsamples decays rapidly,in particular for single
crystals.One speaks of ‘giant ﬂux creep’.This is a strong hint that ﬂux pinning is insufﬁcient at 77 K
and implies that the presently available materials are not yet suited for building magnets cooled by liquid
nitrogen.
Fig.44:Comparison of superconductor magnetisation decay due to ﬂux creep in NbTi at a temperature of 4.2 K,in oriented
grained YBa
2
Cu
3
O
x
at 77 K and in a YBa
2
Cu
3
O
x
single crystal at 60 K [36].
7.SUPERCONDUCTORS IN MICROWAVE FIELDS
Superconductivity in microwave ﬁelds is not treated adequately in standard text books.For this reason
I present in this section a simpliﬁed explanation of the important concepts.A similar treatment can be
found in [37].Superconductors are free from energy dissipation in directcurrent (dc) applications,but
this is no longer true for alternating currents (ac) and particularly not in microwave ﬁelds.The reason
is that the highfrequency magnetic ﬁeld penetrates a thin surface layer and induces oscillations of the
electrons which are not bound in Cooper pairs.The power dissipation caused by the motion of the
unpaired electrons can be characterized by a surface resistance.In copper cavities the surface resistance
is given by
R
surf
=
1
(43)
where is the skin depth and the conductivity of the metal.
The response of a superconductor to an ac ﬁeld can be understood in the framework of the two
ﬂuid model
4
.An ac current in a superconductor is carried by Cooperpairs (the superﬂuid component)
as well as by unpaired electrons (the normal component).Let us study the response to a periodic electric
ﬁeld.The normal current obeys Ohm’s law
J
n
=
n
E
0
exp(i!t) (44)
while the Cooper pairs receive an acceleration m
c
_v
c
= 2e E
0
exp(i!t),so the supercurrent density
becomes
J
s
= i
n
c
2 e
2
m
e
!
E
0
exp(i!t):(45)
If we write for the total current density
J = J
n
+J
s
= E
0
exp(i!t) (46)
4
A similar model is used to explain the unusual properties of liquid helium below 2.17 K in terms of a normal and a
superﬂuid component.
we get a complex conductivity:
=
n
+i
s
with
s
=
2 n
c
e
2
m
e
!
=
1
0
2
L
!
:(47)
The surface resistance is the real part of the complex surface impedance
R
surf
= Re
1
L
(
n
+i
s
)
=
1
L
n
2
n
+
2
s
:(48)
Since
2
n
2
s
at microwave frequencies one can disregard
2
n
in the denominator and obtains R
surf
/
n
=(
L
2
s
).So we arrive at the surprising result that the microwave surface resistance is proportional to
the normalstate conductivity.
The conductivity of a normal metal is given by the classic Drude expression
n
=
n
n
e
2
`
m
e
v
F
(49)
where n
n
is the density of the unpaired electrons,`their mean free path and v
F
the Fermi velocity.The
normal electrons are created by thermal breakup of Cooper pairs.There is an energy gap E
g
= 2(T)
between the BCS ground state and the free electron states.By analogy with the conductivity of an
intrinsic (undoped) semiconductor we get
n
/`exp(E
g
=(2k
B
T)) =`exp((T)=(k
B
T)):(50)
Using 1=
s
=
0
2
L
!and (T) (0) = 1:76k
B
T
c
we ﬁnally obtain for the BCS surface resistance
R
BCS
/
3
L
!
2
`exp(1:76 T
c
=T):(51)
This formula displays two important aspects of microwave superconductivity:the surface resistance
depends exponentially on temperature,and it is proportional to the square of the radio frequency.
Eq.(51) applies if the mean free path`of the unpaired electrons is much larger than the coherence
length .In niobiumthis condition is usually not fulﬁlled and one has to replace
L
in the above equation
by [38]
=
L
p
1 +=`:(52)
Fig.45:The surface resistance of a 9cell TESLA cavity plotted as a function of T
c
=T.The residual resistance of 3 n
corresponds to a quality factor Q
0
= 10
11
.
Combining equations (51) and (52) we arrive at the surprising statement that the surface resistance
does not assume its minimum value when the superconductor is of very high purity (` ) but rather
in the range` .Experimental results [39] and theoretical models [40] conﬁrm this prediction.The
effect is also observed in copper cavities with a thin niobium sputter coating in which the electron mean
free path is in the order of .At 4.2 K the quality factors in the LEP cavities are indeed a factor of two
higher than in pure niobium cavities [41].
In addition to the BCS termthere is a residual resistance caused by impurities,frozenin magnetic
ﬂux or lattice distortions.
R
surf
= R
BCS
+R
res
:(53)
R
res
is temperature independent and amounts to a few n
for a clean niobium surface but may readily
increase if the surface is contaminated.
For niobium the BCS surface resistance at 1.3 GHz amounts to about 800 n
at 4.2 K and drops
to 15 n
at 2 K,see Fig.45.The exponential temperature dependence is the reason why operation at
2 K is essential for achieving high accelerating gradients in combination with very high quality factors.
Superﬂuid helium is an excellent coolant owing to its high heat conductivity.
8.JOSEPHSONEFFECTS
In 1962 B.D.Josephson made a theoretical analysis of the tunneling of Cooper pairs through a thin
insulating layer from one superconductor to another and predicted two fascinating phenomena which
were fully conﬁrmed by experiment.A schematic experimental arrangement is shown in Fig.46.
Fig.46:Schematic arrangement for studying the properties of a Josephson junction.
DC Josephson effect.If the voltage V
0
across the junction is zero there is a dc Cooperpair current which
can assume any value in the range
I
0
< I < I
0
where I
0
is a maximum current that depends on the Cooperpair densities and the area of the junction.
AC Josephson effect.Increasing the voltage of the power supply eventually leads to a nonvanishing
voltage across the junction and then a new phenomenon arises:besides a dc current which however is
now carried by single electrons there is an alternating Cooperpair current
I(t) = I
0
sin(2f
J
t +'
0
) (54)
whose frequency,the socalled Josephson frequency,is given by the expression
f
J
=
2eV
0
2~
:(55)
For a voltage V
0
= 1 V one obtains a frequency of 483.6 MHz.The quantity'
0
is an arbitrary phase.
Equation (55) is the basis of extremely precise voltage measurements.
8.1 Schr
¨
odinger equation of the Josephson junction
The wave functions in the superconductors 1 and 2 are called
1
and
2
.Due to the possibility of
tunneling through the barrier the two Schr¨odinger equations are coupled
i~
@
1
@t
= E
1
1
+K
2
;i~
@
2
@t
= E
2
2
+K
1
:(56)
The quantity K is the coupling parameter.The macroscopic wave functions can be expressed through
the Cooperpair densities n
1
;n
2
and the phase factors
1
=
p
n
1
exp(i'
1
);
2
=
p
n
2
exp(i'
2
):(57)
We insert this into (56) and obtain
_n
1
2
p
n
1
+i
p
n
1
_'
1
exp(i'
1
) =
i
~
[E
1
p
n
1
exp(i'
1
) +K
p
n
2
exp(i'
2
)]
and
_n
2
2
p
n
2
+i
p
n
2
_'
2
exp(i'
2
) =
i
~
[E
2
p
n
2
exp(i'
2
) +K
p
n
1
exp(i'
1
)]:
Now we multiply these equation with exp(i'
1
) resp.exp(i'
2
) and separate the real and imaginary
parts:
_n
1
=
2K
~
p
n
1
n
2
sin('
2
'
1
);
_n
2
=
2K
~
p
n
1
n
2
sin('
1
'
2
) = _n
1
;
_'
1
=
1
~
E
1
+K
r
n
2
n
1
cos('
2
'
1
)
;(58)
_'
2
=
1
~
E
2
+K
r
n
1
n
2
cos('
1
'
2
)
:
For simplicity we consider the case where the two superconductors are identical,so n
2
= n
1
.The
Cooperpair energies E
1
and E
2
differ by the energy gained upon crossing the voltage V
0
:
E
2
= E
1
2eV
0
:
The equations simplify
_n
1
=
2K
~
n
1
sin('
2
'
1
) = _n
2
;
d
dt
('
2
'
1
) =
1
~
(E
2
E
1
) =
2eV
0
~
:(59)
Integrating the second equation (59) yields the Josephson frequency
'
2
(t) '
1
(t) =
2eV
0
~
t +'
0
= 2f
J
t +'
0
:(60)
The Cooperpair current through the junction is proportional to _n
1
.Using (59) and (60) it can be written
as
I(t) = I
0
sin
2eV
0
~
t +'
0
:(61)
There are two cases:
(1) For zero voltage across the junction we get a dc current
I = I
0
sin'
0
which can assume any value between I
0
and +I
0
since the phase'
0
is not speciﬁed.
(2) For V
0
6= 0 there is an ac Cooper–pair current with exactly the Josephson frequency.
8.2 Superconducting quantuminterference
A loop with two Josephson junctions in parallel (Fig.47) exhibits interference phenomena that are
similar to the optical diffraction pattern of a double slit.Assuming zero voltage across the junctions the
total current is
I = I
a
+I
b
= I
0
(sin'
a
+sin'
b
):
When a magnetic ﬂux
mag
threads the area of the loop,the phases differ according to Sec.5 by
'
b
'
a
=
2e
~
I
~
A
~
ds =
2e
~
mag
:
With'
0
= ('
a
+'
b
)=2 we get
'
a
='
0
+
e
~
mag
;'
b
='
0
e
~
mag
and the current is
I = I
0
sin
0
cos
e
~
mag
:(62)
Fig.47:A loop with two Josephson junctions and the observed interference pattern [42].The amplitude modulation is caused
by the ﬁnite width of the junctions.
As a function of the magnetic ﬂux one obtains a typical doubleslit interference pattern as shown
in Fig.47.Adjacent peaks are separated by one ﬂux quantum
mag
=
0
,so by counting ﬂux quanta
one can measure very small magnetic ﬁelds.This is the basic principle of the Superconducting Quantum
Interference Device (SQUID).Technically one often uses superconducting rings with a single weak link
which acts as a Josephson junction.Flux transformers are applied to increase the effective area and
improve the sensitivity.
A FREE ENERGYIN THERMODYNAMICS
To illustrate the purpose of the free energy I consider ﬁrst an ideal gas.The internal energy is the sumof
the kinetic energies of all atoms
U =
N
X
i=1
m
2
v
2
i
=
3
2
N k
B
T (63)
and depends only on temperature but not on volume.The ﬁrst law of thermodynamics describes energy
conservation:
dU = Q+W:(64)
The internal energy increases either by adding heat Qor mechanical work W = pdV to the gas.For
a reversible process one has Q = T dS where S is the entropy.Now consider an isothermal expansion
of the gas.Thereby the gas transforms heat into mechanical work:
dU = 0 for T = const ) Q = W = pdV:(65)
The gas produces mechanical work but its internal energy does not change,hence U is not an ade
quate variable to describe the process.What is the correct energy variable?We will see that this is the
Helmholtz free energy,given by
F = U T S ) dF = dU SdT TdS = W SdT:(66)
For an isothermal expansion (dT = 0) we get dF = W,i.e.dF = pdV:the work produced by the
gas is identical to the reduction of its free energy.
Now we consider a magnetic material of permeability inside a coil which generates a ﬁeld H.
The magnetization is
~
M = ( 1)
~
H.Its potential energy (per unit volume) in the magnetic ﬁeld is
E
pot
=
0
~
M
~
H:(67)
If the magnetization changes by
~
dM the work is W =
0
~
dM
~
H.Deﬁning again the Helmholtz free
energy by eq.(66) we get by analogy with the ideal gas dF = W,hence F can in fact be used to
describe the thermodynamics of magnetic materials in magnetic ﬁelds.One drawback is,however,that
the magnetization of a substance cannot be directly varied by the experimenter.What can be varied at
will is the magnetic ﬁeld H,namely by choosing the coil current.For this reason another energy function
is more appropriate,the Gibbs free energy
G = F
0
~
M
~
H = U T S
0
~
M
~
H:(68)
For an isothermal process we get dG =
0
~
M
~
dH.Let us apply this to a superconductor in the
Meissner phase.Then = 0 and
~
M =
~
H from which follows
dG
sup
=
0
M(H)dH =
0
2
d(H
2
) ) G
sup
(H) = G
sup
(0) +
0
2
H
2
:(69)
This equation is used in Sect.3.
B THE FORMATIONOF A COOPERPAIR
To illustrate the spirit of the BCS theory I will present the mathematics of Cooperpair formation.Let us
consider a metal at T = 0.The electrons ﬁll all the energy levels below the Fermi energy while all levels
above E
F
are empty.The wave vector and the momentum of an electron are related by
~p = ~
~
k:
In the threedimensional k space the Fermi sphere has a radius k
F
=
p
2m
e
E
F
=~.To the fully occupied
Fermi sphere we add two electrons of opposite wave vectors
~
k
1
=
~
k
2
whose energy E
1
= E
2
=
~
2
k
2
1
=(2m
e
) is within the spherical shell (see Figs.20,23)
E
F
< E
1
< E
F
+~!
D
:(70)
From Sect.4 we know that ~!
D
is the largest energy quantum of the lattice vibrations.The interaction
with the ‘sea’ of electrons inside the Fermi sphere is neglected except for the Pauli Principle:the two
additional electrons are forbidden to go inside because all levels below E
F
are occupied.Under this
assumption the two electrons together have the energy 2E
1
> 2E
F
.Now the attractive force provided
by the lattice deformation is taken into consideration.Following Cooper [18] we must demonstrate that
the two electrons then forma bound system,a ‘Cooper pair’,whose energy drops below twice the Fermi
energy
E
pair
= 2E
F
E < 2E
F
:
The Schr¨odinger equation for the two electrons reads
~
2
2m
e
(r
2
1
+r
2
1
) (~r
1
;~r
2
) +V (~r
1
;~r
2
) (~r
1
;~r
2
) = E
pair
(~r
1
;~r
2
) (71)
where V is the interaction potential due to the dynamical lattice polarisation.In the simple case of
vanishing interaction,V = 0,the solution of (71) is the product of two plane waves
(~r
1
;~r
2
) =
1
p
L
3
exp(i
~
k
1
~r
1
)
1
p
L
3
exp(i
~
k
2
~r
2
) =
1
L
3
exp(i
~
k ~r)
with
~
k
1
=
~
k
2
=
~
k the kvector,~r = ~r
1
~r
2
the relative coordinate and L
3
the normalisation volume.
The most general solution of Eq.(71) with V = 0 is a superposition of such functions
(~r) =
1
L
3
X
~
k
g(
~
k) exp(i
~
k ~r) (72)
with the restriction that the coefﬁcients g(
~
k) vanish unless E
F
~
2
k
2
=2m
e
E
F
+~!
D
.This function
is certainly not an exact solution of the equation (71) with V 6= 0 but for a weak potential it can be used
to obtain the energy E
pair
in ﬁrst order perturbation theory.For this purpose we insert (72) into Eq.(71):
1
L
3
X
~
k
0
g(
~
k
0
)
"
~
2
k
0
2
m
e
+V (~r) E
pair
#
exp(i
~
k
0
~r) = 0:
This equation is multiplied by exp(i
~
k ~r) and integrated,using the orthogonality relations
1
L
3
Z
exp
i(
~
k
0
~
k) ~r
d
3
r =
~
k
~
k
0
with
~
k
~
k
0
=
1 for
~
k =
~
k
0
0 otherwise:
Introducing further the transition matrix elements of the potential V
V
~
k
~
k
0
=
Z
exp
i(
~
k
~
k
0
) ~r
V (~r)d
3
r (73)
one gets a relation among the coefﬁcients of the expansion (72)
g(
~
k)
~
2
k
2
m
e
E
pair
=
1
L
3
X
~
k
0
g(
~
k
0
)V
~
k
~
k
0
:(74)
The matrix element V
~
k
~
k
0
describes the transition from the state (
~
k;
~
k) to any other state (
~
k
0
;
~
k
0
) in
the spherical shell of thickness ~!
D
around the Fermi sphere.Cooper and later Bardeen,Cooper and
Schrieffer made the simplest conceivable assumption on these matrix elements,namely that they are all
equal.
V
~
k
~
k
0
= V
0
for E
F
<
~
2
k
2
2m
e
;
~
2
k
02
2m
e
< E
F
+~!
D
(75)
and V
~
k
~
k
0
= 0 elsewhere.The negative value ensures attraction.With this extreme simpliﬁcation the
righthand side of Eq.(74) is no longer
~
k dependent but becomes a constant
1
L
3
X
~
k
0
g(
~
k
0
)V
~
k
~
k
0
=
V
0
L
3
X
~
k
0
g(
~
k
0
) = A:(76)
Then Eq.(74) yields for the coefﬁcients
g(
~
k) =
A
~
2
k
2
=m
e
E
pair
=
A
~
2
k
2
=m
e
2E
F
+E
:
The constant A is still unknown.We can eliminate it by summing this expression over all
~
k and using
(76) once more
X
~
k
g(
~
k) = A
L
3
V
0
fromwhich follows
A
L
3
V
0
=
X
~
k
A
~
2
k
2
=m
e
2E
F
+E
:
Dividing by A leads to the important consistency relation
1 =
V
0
L
3
X
~
k
1
~
2
k
2
=m
e
2E
F
+E
:(77)
The sum extends over all
~
k vectors in the shell between E
F
and E
F
+~!
D
.Since the states are very
densely spaced one can replace the summation by an integration
1
L
3
X
~
k
!
1
(2)
3
Z
d
3
k!
Z
N(E)dE
where N(E) is the density of singleelectron states for a deﬁnite spin orientation.(The states with
opposite spin orientation must not be counted because a Cooper pair consists of two electrons of opposite
spin).The integration spans the narrow energy range [E
F
;E
F
+ ~!
D
] so N(E) can be replaced by
N(E
F
) and taken out of the integral.Introducing a scaled energy variable
= E E
F
=
~
2
k
2
2m
e
E
F
formula (77) becomes
1 = V
0
N(E
F
)
Z
~!
D
0
d
2 +E
:(78)
The integral yields
1
2
ln
E +2~!
D
E
:
The energy shift is then
E =
2~!
D
exp(2=(V
0
N(E
F
)) 1
:
For small interaction potentials (V
0
N(E
F
) 1) this leads to the famous Cooper formula
E = 2~!
D
exp
2
V
0
N(E
F
)
:(79)
Except for a factor of 2 the same exponential appears in the BCS equations for the energy gap and the
critical temperature.
References
[1] W.Buckel,Supraleitung,4.Auﬂage,VCH Verlagsgesellschaft,Weinheim 1990
[2] D.R.Tilley & J.Tilley,Superﬂuidity and Superconductivity,Third Edition,Institute of Physics
Publishing Ltd,Bristol 1990
[3] H.K.Onnes,Akad.van Wetenschappen (Amsterdam) 14,113,818 (1911)
[4] J.File and R.G.Mills,Phys.Rev.Lett.10,93 (1963)
[5] M.N.Wilson,private communication
[6] W.Meissner and R Ochsenfeld,Naturwiss.21,787 (1933)
[7] F.London and H.London,Z.Phys.96,359 (1935)
[8] J.Bardeen,L.N.Cooper and J.R.Schrieffer,Phys.Rev.108,1175 (1957)
[9] V.L.Ginzburg and L.D.Landau,JETP USSR 20,1064 (1950)
[10] L.P.Gorkov,Sov.Phys.JETP 9,1364 (1960),JETP 10,998 (1960)
[11] A.A.Abrikosov,Sov.Phys.JETP 5,1174 (1957)
[12] U.Essmann and H.Tr¨auble,Phys.Lett.24A,526 (1967) and Sci.Am.224,March 1971
[13] B.D.Josephson,Phys.Rev.Lett.1,251 (1962)
[14] J.D.Livingston,Phys.Rev.129,1943 (1963)
[15] N.E.Phillips,Phys.Rev.134,385 (1965)
[16] Th.Schilcher,Diploma Thesis,Hamburg 1994,unpublished
[17] M.N.Wilson,Superconducting Magnets,Oxford University Press 1997
[18] L.N.Cooper,Phys.Rev.104,1189 (1956)
[19] H.Ibach and H.L¨uth,Solid State Physics,2nd Edition,SpringerVerlag,Berlin 1996
[20] Y.Aharonov and D.Bohm,Phys.Rev.115,485 (1955)
[21] G.M¨ollenstedt and W.Bayh,Phys.Bl.18,229 (1962)
[22] A.Tonomura,Phys.Today,April 1990
[23] R.Doll and M.N¨abauer,Phys.Rev.Lett.7,51 (1961)
[24] B.S.Deaver and W.M.Fairbank,Phys.Rev.Lett.7,43 (1961)
[25] H.Rietschel,Phys.Bl.46,419 (1990)
[26] C.E.Gough et al.,Nature 326,855 (1987)
[27] G.T.Lee et al.,Physica C 161,195 (1989)
[28] Y.B.Kim,C.F.Hempstead and A.R.Strnad,Phys.Rev.139,A1163 (1965)
[29] Y.B.Kim,C.F.Hempstead and A.R.Strnad,Phys.Rev.Lett.9,306 (1962)
[30] P.W.Anderson,Phys.Rev.Lett.9,309 (1962)
[31] K.H.Mess,P.Schm¨user,S.Wolff,Superconducting Accelerator Magnets,World Scientiﬁc,Sin
gapore,1996
[32] H.Br¨uck et al.,Contribution to the European Accelerator Conference,Nice 1990
[33] M.Halemeyer et al.,IEEE Trans.Appl.Supercond.Vol.3,No.1,168 (1993)
[34] A.P.Verweij and H.H.J.ten Kate,IEEE Trans.ASC5 (1995) 404
[35] L.Krempaski and C.Schmidt,Appl.Phys.Lett.66 (1995) 1545,and J.Appl.Phys.78 (1995) 5800
[36] C.Keller et al.,Cryogenics 30,410 (1990)
[37] H.Padamsee,J.Knobloch and T.Hays,RF Superconductivity for Accelerators,John Wiley,New
York 1998
[38] B.Bonin,CERNAccelerator School Superconductivity in Particle Accelerators,CERN 9603,ed.
S.Turner,Hamburg (1995)
[39] F.Palmer,Proc.3rd Workshop on RF Superconductivity,K.Shephard (ed.),Argonne Natl.Lab.
1988,p.309
[40] J.Halbritter,Z.Physik 238 (1970) 466
[41] C.Benvenuti et al.,Proc.PAC91,San Francisco (1991),p.1023.
[42] R.C.Jaklevic et al.Phys.Rev.140,A1628 (1965)
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Comments 0
Log in to post a comment